footprint ". |
has been written about the origins of the 'original' shino glazes. In this article
I would like to give a brief outline of these. Also looking at the glazes now
known as carbon trapping or 'American' shino, and how these recipes may be formulated
using UK materials. The mechanics of how this glaze feature may be developed through
glaze composition and firing cycles. Using fuel burning kilns i.e. Gas, oil and
wood, how carbon trapping may be encouraged as a decorative ceramic surface. Also
a brief look at high flux content clays in protracted anagama wood firings and
there ability to trap subtle carbon patterns and markings beneath the natural
ash glaze and soda fluxed surfaces.
It has been speculated that the type of glazes known as shino were developed in
response to Japanese tea masters' demand for Chinese white porcelain wares in
the Momoyama period (1573 - 1615). This cream white glaze was highly prized for
Tea ceremony wares. Feldspathic materials from the Mino area of Japan mixed with
ash, and clay created a viscous white glaze which had a tendency to crawl and
pin hole, these qualities have been and predominantly still are viewed as faults
in Western eyes but viewed in the light of desires by tea masters to use utensils
which bore an organic, natural beauty they were admired as another integral aesthetic
facet of the object. Several classifications of shino were identified: Plain shino
(Muji shino), Picture shino (e-shino), Crimson shino (beni shino), Red shino (aka
shino), Grey shino (nezumi shino) and marbled shino (neriage shino), each having
a subtly different surface. Some of these glazes were applied over iron bearing
slips or delicate Iron brush work. Due to the firing techniques used, iron bled
through the glaze creating exquisite surfaces.
The family of glazes now known as American shino were developed by Virginia Wirt
in the early seventies, as part of a project which was set at the University of
Minnesota, "to try and replicate early Japanese glazes". Wirt is widely
acknowledged as the first to add soda ash to a shino type glaze in order to attempt
to utilise carbon trapping. From this beginning many recipes have been created
which push forward this decorative technique notably by Malcolm Davis, Dick Lehman,
Jack Troy, Jeff Oestrich and Cris Gustin, to name but a few, all from the USA.
It is arguable as to how reminiscent these glazes actually are to the original
momoyama glazes however there are some very similar molecular similarities in
there composition. The colours which these glazes produce are within the same
pallet with the added dimension of areas shaded by the entrapment of carbon.
UK materials offer some wonderful scope for this type of glaze. The main common
material is soda ash; a low temperature flux: this may be added to other higher
temperature fluxes such as, nepheline syenite or soda feldspar. Nepheline syenite
melts at a lower temperature than soda feldspar so may provide an advantage in
the trapping process. An addition of ball clay will give a rudimentary starting
point for further experimentation. High iron bearing ball clays such as Hymod
AT will give a correspondingly darker colouration to the glaze burning to darker
reds and oranges, lighter ball clays such as Hyplas 71 will give lighter blushes
of colour. Red earthenware powders or locally dug low firing clays may be added
to the glaze to introduce higher iron in addition to other possibly beneficial
impurities. I prefer to introduce the bulk of the iron in this way using a lighter
firing ball clay as a base. It is interesting to test with several dug clays to
see what differences become apparent in the finished glaze. These clays should
be dried crushed and turned into a slip. The slip is then worked through an 80's
sieve and re-dried and crushed the dug clay can then be added as a dry material
to the dry glaze mix. Several ball clays have been used in tests some with higher
carbon contents than others (blue ball clays and black ball clays), I found no
significant differences in the carbon trapping qualities of the resulting glazes.
The addition of spodumene, petalite or lepidolite, all lithium feldspars which
contain soluble alkalies, can enhance the colour of some glazes as well as producing
a hard durable surface, they may also reduce crazing in the glaze if this is desirable.
I have carried out many tests using porcelain, this can lead to some striking
black and white contrast. A very small percentage of iron bearing clay may be
added either to the porcelain body itself or as a very thin wash to encourage
oranges, pinks and reds within the glaze but still maintain the translucent bright
quality of the body.
the firings which have been carried out have been undertaken using kilns at The
Ceramics program at Loughborough University School of Art and Design and the anagama
kiln at Wysing Arts near Bourne in Cambridgeshire.
Carbon trapping in these shino type glazes can be elusive, the position of pots
in the kiln and cycle of reduction appear to be key ingenerating the range of
carbon spotting, haloing and lining which can appear. Also the orange, red and
pink colourations of the main body of the glaze also responds to these. The clay
body on which the glazes are applied greatly effects the glaze finish.
Most carbon trapping glazes contain a quantity of soda ash. This material is soluble,
and starts its melt as low as 800 degrees C. When a piece has been glazed with
a high soda ash glaze, crystals may be seen to appear on the surface creating
beautiful patterns in there own right during the drying process. This crystal
accumulation may be controlled through allowing areas of the pots to dry at differing
rates or applying resists toinhibit the crystal growth. It is important that these
crystals are not disturbed while handling pots post glazing, as these areas are
where the strongest potential is for trapping carbon. Soda ash solution may also
be painted over the surface of the glaze to promote more intense localised crystal
formation. Due to the soluble nature of soda ash if a glaze is applied just as
a liner glaze the soda can migrate through the ceramic body and promote flame
flashing and carbon trapping on the exterior of the work. In order to facilitate
this, the work should be given a very low bisc to allow maximum porosity through
which the soda can migrate.
the reduction firing, fine particles of carbon build up on the surface of the
pot and settle between the soda crystals. When these fine soda crystals start
to melt they trap the carbon against the body of the unmelted glaze. When the
main body of the glaze starts to melt the carbon present becomes encased in the
main glaze melt. It is for this reason that the reduction cycle for this type
of glaze firing begins as low as orton cone 013 (850C) or even slightly earlier.
I have started reducing as low as cone 015 (800) without any detrimental effects.
A very heavy reduction at this stage gives the best chance of collecting carbon.
It therefore follows that firing with a fuel that is capable of generating a lot
of soot if inefficiently burned will give the largest carbon build up. Oil and
wood produce the most carbon in early reduction.
A natural draught gas kiln needs to be closed up tight (dampers fully in) to achieve
sufficient reduction, I hold this reduction for about two hours. If it is an internal
kiln the room must be very well ventilated to avoid the risk of exposure to carbon
monoxide. In anagama, the fire box is stoked with larger amounts of wood. A good
bed of hard wood coals, allows more control over the stoking of softwood to achieve
a really smoky atmosphere. The under grate air and lower stoke holes are also
closed to produce a slow rolling flame through the kiln. In the oil fired kiln
just a small adjustment to the damper can achieve a strong, smoky reduction. After
this first period of heavy reduction a constant heavy/ medium reduction is kept
until close to the start of the main melt of the glaze. In the case of the anagama
the cycle is between very heavy reduction on the stoke changing gradually to oxidation
as the stoke burns down giving off heat, and then back into reduction on the next
of the carbon trapping glazes which I use, benefit from a cone 10 to 12 firing
although I have fired to lower temperatures these carbon trapping shino glazes
like a good soak at lower temperature (cone 9), to achieve a good melt. In some
instances the soda ash flux can appear as a rather unattractive (to my eyes) green
glass on the surface of the glaze I feel that firing higher and for as long as
possible gives the best results. A longer duration to the firing and a period
of very heavy reduction followed by a period of oxidation (10 minutes or so),
right at the end of the firing promotes orange flashes in the glaze due to very
fine iron particle suspended in the glaze matrix. This system works well in gas
or oil kilns, however with anagama I tend to reduction cool on the last stoke
i.e. fill the firebox with wood, cap the chimney and clam up the stoke and spy
holes, this produces a final heavy reduction and causes the final stoke to burn
down slowly. I have had equally good results from all methods.
Undoubtedly the finest results have been achieved in wood firings due to the quantities
of smoke, ash and the overall duration of the various stages of the firing (three
to five days overall). Duration allows a thorough melt of the glaze and the fluctuations
in atmosphere generate wonderful colours due to interactions of iron in the body.
My shinos work very well if placed in saggars in this type of firing. A perforated
saggar which allows a small amount of flame to impinge on the pot inside can result
in black carbon spots which correlate to the positions of the holes, satin matt
surfaces on the glaze rather than glassy due to high alumina to silica ratio and
crystallization in the cooling can introduce wonderful surface drama with a fluid
natural ash glaze settled on the top. Equally beautiful but different results
have been achieved in the gas and oil kilns. The overall glaze surface tends to
be less flawed with the glaze taking on a wonderful soft lustrous quality with
more even distributions of carbon markings responding to subtleties in the forms.
All of the bodies which I use contain a fairly high nepheline syenite flux content
(up to 22%). This can create a fluxed glassy surface on the finished pieces, in
extended wood firing. These clays also work well in all other firings and add
to the fluxing action of the glazes, creating a strong clay glaze interface.
The mechanics of these bodies ability to trap carbon under this final glassy surface,
in extended firings, relies also in part on alkalies carried by the fire flames
in the very early stages of a firing as well as the migration of soluble soda
in the body. In a similar way to that of carbon trap shino glazes, the alkali
content in fly ash and other gases emitted from the burning fuel interact with
the ceramic surface of the pots, combining with soda still present from the nepheline
syenite in the body. The migrated soda layer melts early on in the firing and
in this way traps the carbon when the body becomes glassy. High flux porcelains
have been seen to take on a shine in the very early stages of a firing (cone 06).
Pieces which have been placed towards the rear of the kiln have shown some subtle
carbon trapping under the fluxed body surface due to a build up of carbon when
the front temperature indicates the start of reduction but the back of the kiln
could still be as low as cone 017 (700ish).
To conclude, in this article it
has only been possible to give a brief outline to the potential of these types
of glaze and carbon trapping in general. As always, the form of an object is its
main strength, but the ability of this type of glazing to emphasise marks and
reflect the relationship to other work in the kiln introduces a subtle element
of serendipity to the finished object. There is much scope left for further exploration
into the use of soda ash and other soluble materials to create surface finishes.
Also with our wealth of native Devon and Dorset ball clays as well as numerous
local clay deposits, new surfaces are waiting to be explored and utilised. The
subtlety, warmth and empathy to form which carbon trapping glazes can impart makes
these glazes a useful addition to the ceramic pallet. There is also the magic
factor which allows the maker to lose control and hand it over to the fire. Forcing
preconceptions of the objects we produce to be challenged.
1 Orton cone 10 - 12 reduction
syenite - 42.5
Soda feldspar - 10.25
Hywite HK2 Ball clay - 14.32 (can
be substituted for Hyplas)
China clay - 9.5
Soda ash - 17.9
to a white/ orange glaze with grey to black carbon trapping.
2 Orton cone 10 - 12 reduction.
syenite - 50
Spodumene - 20
China clay - 12
AT Ball clay - 8
ash - 12
Red clay powder - 3
to a rich red to dark orange to cream with strong carbon trapping. Can give a
beautiful lustrous gold.
3 Orton cone 10 -12 reduction.
syenite - 52
Prima ball clay - 14
China clay - 10
Soda ash - 13
Red clay - 2
rich orange carbon trapping glaze very sensitive to firing atmosphere.
stoneware of Japan: shino and
oribe". Ryoji Kuroda & Takeshi Murayama.
shino". Mel Jacobson. Ceramics Monthly
Fires: Another face of shino". Jim Robinson. The studio Potter: Vol. 21 No.
1 December 1992
Stoneware and Porcelain". Jack Troy. Chilton. 1995